#------------------------------------------------------------------------------
#$Date: 2016-03-21 01:21:50 +0200 (Mon, 21 Mar 2016) $
#$Revision: 178377 $
#$URL: svn://www.crystallography.net/cod/cif/4/00/13/4001369.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4001369
loop_
_publ_author_name
'Ehora, Ghislaine'
'Renard, Catherine'
'Daviero-Minaud, Sylvie'
'Mentré, Olivier'
_publ_section_title
;
 New BaCoO3-\dPolytypes by Rational Substitution of O2-for F-
;
_journal_issue                   12
_journal_name_full               'Chemistry of Materials'
_journal_page_first              2924
_journal_paper_doi               10.1021/cm070576o
_journal_volume                  19
_journal_year                    2007
_chemical_formula_moiety         Ba6Co6FO16
_chemical_formula_sum            'Ba6 Co6 F O16'
_chemical_formula_weight         1452.62
_chemical_name_common            'barium cobalt oxyfluorure'
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           187
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P -6 2'
_symmetry_space_group_name_H-M   'P -6 m 2'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   5.6683(5)
_cell_length_b                   5.6683(5)
_cell_length_c                   14.277(3)
_cell_measurement_temperature    293(2)
_cell_volume                     397.26(10)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.972
_diffrn_measured_fraction_theta_max 0.972
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0303
_diffrn_reflns_av_sigmaI/netI    0.0242
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            2137
_diffrn_reflns_theta_full        28.04
_diffrn_reflns_theta_max         28.04
_diffrn_reflns_theta_min         2.85
_exptl_absorpt_coefficient_mu    20.776
_exptl_absorpt_process_details   Sadabs
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    6.072
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             635
_exptl_crystal_size_max          0.3
_exptl_crystal_size_mid          0.2
_exptl_crystal_size_min          0.2
_refine_diff_density_max         0.951
_refine_diff_density_min         -0.984
_refine_diff_density_rms         0.164
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   -0.06(10)
_refine_ls_extinction_coef       0.0074(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.194
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     45
_refine_ls_number_reflns         415
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.192
_refine_ls_R_factor_all          0.0164
_refine_ls_R_factor_gt           0.0160
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0106P)²+0.4052P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0346
_refine_ls_wR_factor_ref         0.0348
_reflns_number_gt                410
_reflns_number_total             415
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cm070576osi20070301_112145.cif
_cod_data_source_block           ba6co6f
_cod_original_cell_volume        397.25(9)
_cod_original_sg_symbol_H-M      P-6m2
_cod_database_code               4001369
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'x, y, -z'
'-y, x-y, -z'
'-x+y, -x, -z'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'
'-y, -x, -z'
'-x+y, y, -z'
'x, x-y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ba1 Ba 1.0000 1.0000 0.81007(5) 0.00935(17) Uani 1 6 d S
Ba2 Ba 0.3333 0.6667 0.64792(4) 0.00915(18) Uani 1 6 d S
Ba3 Ba 0.6667 0.3333 1.0000 0.0219(3) Uani 1 12 d S
Ba4 Ba 1.0000 1.0000 0.5000 0.0118(2) Uani 1 12 d S
Co1 Co 0.6667 0.3333 0.75623(10) 0.0065(3) Uani 1 6 d S
Co2 Co 0.6667 0.3333 0.58424(11) 0.0065(3) Uani 1 6 d S
Co3 Co 0.3333 0.6667 0.87855(10) 0.0091(3) Uani 1 6 d S
O1 O 0.8147(6) 0.6294(11) 0.6689(3) 0.0093(11) Uani 1 2 d S
O2 O 0.5071(7) 0.4929(7) 0.8361(3) 0.0129(9) Uani 1 2 d S
O3 O 0.9664(16) 0.4832(8) 0.5000 0.0100(15) Uani 1 4 d S
O4 O 0.293(5) 0.586(10) 0.0000 0.07(2) Uani 0.33 4 d SP
F1 F 1.0000 1.0000 1.0000 0.095(8) Uani 1 12 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
F1 Ba1 O1 137.92(10) . .
F1 Ba1 O1 137.92(10) . 3_675
O1 Ba1 O1 70.95(16) . 3_675
F1 Ba1 O1 137.92(10) . 2_765
O1 Ba1 O1 70.95(16) . 2_765
O1 Ba1 O1 70.95(16) 3_675 2_765
F1 Ba1 O2 82.53(8) . 1_665
O1 Ba1 O2 131.57(14) . 1_665
O1 Ba1 O2 96.48(11) 3_675 1_665
O1 Ba1 O2 60.86(11) 2_765 1_665
F1 Ba1 O2 82.53(8) . .
O1 Ba1 O2 60.86(11) . .
O1 Ba1 O2 96.48(11) 3_675 .
O1 Ba1 O2 131.57(14) 2_765 .
O2 Ba1 O2 164.80(17) 1_665 .
F1 Ba1 O2 82.53(8) . 2_765
O1 Ba1 O2 96.48(11) . 2_765
O1 Ba1 O2 131.57(14) 3_675 2_765
O1 Ba1 O2 60.86(11) 2_765 2_765
O2 Ba1 O2 56.6(3) 1_665 2_765
O2 Ba1 O2 118.34(4) . 2_765
F1 Ba1 O2 82.53(8) . 3_675
O1 Ba1 O2 131.57(13) . 3_675
O1 Ba1 O2 60.86(11) 3_675 3_675
O1 Ba1 O2 96.48(11) 2_765 3_675
O2 Ba1 O2 62.2(3) 1_665 3_675
O2 Ba1 O2 118.34(4) . 3_675
O2 Ba1 O2 118.34(4) 2_765 3_675
F1 Ba1 O2 82.53(8) . 3_665
O1 Ba1 O2 60.86(11) . 3_665
O1 Ba1 O2 131.57(14) 3_675 3_665
O1 Ba1 O2 96.48(11) 2_765 3_665
O2 Ba1 O2 118.34(4) 1_665 3_665
O2 Ba1 O2 56.6(3) . 3_665
O2 Ba1 O2 62.2(3) 2_765 3_665
O2 Ba1 O2 164.80(17) 3_675 3_665
F1 Ba1 O2 82.53(8) . 2_665
O1 Ba1 O2 96.48(12) . 2_665
O1 Ba1 O2 60.86(11) 3_675 2_665
O1 Ba1 O2 131.57(13) 2_765 2_665
O2 Ba1 O2 118.34(4) 1_665 2_665
O2 Ba1 O2 62.2(3) . 2_665
O2 Ba1 O2 164.80(17) 2_765 2_665
O2 Ba1 O2 56.6(3) 3_675 2_665
O2 Ba1 O2 118.34(4) 3_665 2_665
F1 Ba1 Co1 103.22(2) . 1_565
O1 Ba1 Co1 99.00(6) . 1_565
O1 Ba1 Co1 34.71(10) 3_675 1_565
O1 Ba1 Co1 99.00(6) 2_765 1_565
O2 Ba1 Co1 93.07(13) 1_665 1_565
O2 Ba1 Co1 93.07(13) . 1_565
O2 Ba1 Co1 148.60(13) 2_765 1_565
O2 Ba1 Co1 35.13(12) 3_675 1_565
O2 Ba1 Co1 148.60(13) 3_665 1_565
O2 Ba1 Co1 35.13(12) 2_665 1_565
F1 Ba1 Co1 103.22(2) . .
O1 Ba1 Co1 34.71(10) . .
O1 Ba1 Co1 99.00(6) 3_675 .
O1 Ba1 Co1 99.00(6) 2_765 .
O2 Ba1 Co1 148.60(13) 1_665 .
O2 Ba1 Co1 35.13(12) . .
O2 Ba1 Co1 93.07(13) 2_765 .
O2 Ba1 Co1 148.60(13) 3_675 .
O2 Ba1 Co1 35.13(12) 3_665 .
O2 Ba1 Co1 93.07(13) 2_665 .
Co1 Ba1 Co1 114.934(19) 1_565 .
O3 Ba2 O3 68.4(2) 1_455 3_675
O3 Ba2 O3 68.4(2) 1_455 2_655
O3 Ba2 O3 68.4(2) 3_675 2_655
O3 Ba2 O1 128.08(16) 1_455 3_675
O3 Ba2 O1 60.09(11) 3_675 3_675
O3 Ba2 O1 96.98(9) 2_655 3_675
O3 Ba2 O1 96.98(9) 1_455 2_665
O3 Ba2 O1 60.09(11) 3_675 2_665
O3 Ba2 O1 128.08(16) 2_655 2_665
O1 Ba2 O1 52.3(2) 3_675 2_665
O3 Ba2 O1 60.09(11) 1_455 1_455
O3 Ba2 O1 96.98(9) 3_675 1_455
O3 Ba2 O1 128.08(16) 2_655 1_455
O1 Ba2 O1 118.91(3) 3_675 1_455
O1 Ba2 O1 67.0(2) 2_665 1_455
O3 Ba2 O1 60.09(11) 1_455 3_565
O3 Ba2 O1 128.08(16) 3_675 3_565
O3 Ba2 O1 96.98(9) 2_655 3_565
O1 Ba2 O1 165.87(17) 3_675 3_565
O1 Ba2 O1 118.91(3) 2_665 3_565
O1 Ba2 O1 52.3(2) 1_455 3_565
O3 Ba2 O1 96.98(9) 1_455 2_655
O3 Ba2 O1 128.08(16) 3_675 2_655
O3 Ba2 O1 60.09(11) 2_655 2_655
O1 Ba2 O1 118.91(3) 3_675 2_655
O1 Ba2 O1 165.87(18) 2_665 2_655
O1 Ba2 O1 118.91(3) 1_455 2_655
O1 Ba2 O1 67.0(2) 3_565 2_655
O3 Ba2 O1 128.08(16) 1_455 .
O3 Ba2 O1 96.98(9) 3_675 .
O3 Ba2 O1 60.09(11) 2_655 .
O1 Ba2 O1 67.0(2) 3_675 .
O1 Ba2 O1 118.91(3) 2_665 .
O1 Ba2 O1 165.87(18) 1_455 .
O1 Ba2 O1 118.91(3) 3_565 .
O1 Ba2 O1 52.3(2) 2_655 .
O3 Ba2 O2 144.71(9) 1_455 2_665
O3 Ba2 O2 107.1(2) 3_675 2_665
O3 Ba2 O2 144.71(9) 2_655 2_665
O1 Ba2 O2 55.49(12) 3_675 2_665
O1 Ba2 O2 55.49(12) 2_665 2_665
O1 Ba2 O2 86.89(9) 1_455 2_665
O1 Ba2 O2 110.79(13) 3_565 2_665
O1 Ba2 O2 110.79(13) 2_655 2_665
O1 Ba2 O2 86.89(9) . 2_665
O3 Ba2 O2 107.1(2) 1_455 3_565
O3 Ba2 O2 144.71(9) 3_675 3_565
O3 Ba2 O2 144.71(9) 2_655 3_565
O1 Ba2 O2 110.79(13) 3_675 3_565
O1 Ba2 O2 86.89(9) 2_665 3_565
O1 Ba2 O2 55.49(12) 1_455 3_565
O1 Ba2 O2 55.49(12) 3_565 3_565
O1 Ba2 O2 86.89(9) 2_655 3_565
O1 Ba2 O2 110.79(13) . 3_565
O2 Ba2 O2 55.32(18) 2_665 3_565
O3 Ba2 O2 144.71(9) 1_455 .
O3 Ba2 O2 144.71(9) 3_675 .
O3 Ba2 O2 107.1(2) 2_655 .
O1 Ba2 O2 86.89(9) 3_675 .
O1 Ba2 O2 110.79(13) 2_665 .
O1 Ba2 O2 110.79(13) 1_455 .
O1 Ba2 O2 86.89(9) 3_565 .
O1 Ba2 O2 55.49(11) 2_655 .
O1 Ba2 O2 55.49(12) . .
O2 Ba2 O2 55.32(18) 2_665 .
O2 Ba2 O2 55.32(18) 3_565 .
O2 Ba3 O2 147.70(10) 6_667 2_655
O2 Ba3 O2 57.6(2) 6_667 5_657
O2 Ba3 O2 112.4(2) 2_655 5_657
O2 Ba3 O2 112.4(3) 6_667 3_665
O2 Ba3 O2 57.6(2) 2_655 3_665
O2 Ba3 O2 147.70(10) 5_657 3_665
O2 Ba3 O2 147.70(10) 6_667 .
O2 Ba3 O2 57.6(2) 2_655 .
O2 Ba3 O2 147.70(10) 5_657 .
O2 Ba3 O2 57.6(2) 3_665 .
O2 Ba3 O2 57.6(2) 6_667 4_557
O2 Ba3 O2 147.70(10) 2_655 4_557
O2 Ba3 O2 57.6(2) 5_657 4_557
O2 Ba3 O2 147.70(10) 3_665 4_557
O2 Ba3 O2 112.4(2) . 4_557
O2 Ba3 O4 56.44(15) 6_667 3_666
O2 Ba3 O4 109.3(4) 2_655 3_666
O2 Ba3 O4 109.3(4) 5_657 3_666
O2 Ba3 O4 56.44(15) 3_665 3_666
O2 Ba3 O4 102.9(5) . 3_666
O2 Ba3 O4 102.9(5) 4_557 3_666
O2 Ba3 O4 56.44(14) 6_667 1_656
O2 Ba3 O4 102.9(5) 2_655 1_656
O2 Ba3 O4 102.9(5) 5_657 1_656
O2 Ba3 O4 56.44(14) 3_665 1_656
O2 Ba3 O4 109.3(4) . 1_656
O2 Ba3 O4 109.3(4) 4_557 1_656
O4 Ba3 O4 12.7(17) 3_666 1_656
O2 Ba3 O4 109.3(4) 6_667 3_556
O2 Ba3 O4 56.44(15) 2_655 3_556
O2 Ba3 O4 56.44(15) 5_657 3_556
O2 Ba3 O4 109.3(4) 3_665 3_556
O2 Ba3 O4 102.9(5) . 3_556
O2 Ba3 O4 102.9(5) 4_557 3_556
O4 Ba3 O4 132.7(17) 3_666 3_556
O4 Ba3 O4 120.000(2) 1_656 3_556
O2 Ba3 O4 102.9(5) 6_667 2_656
O2 Ba3 O4 56.44(14) 2_655 2_656
O2 Ba3 O4 56.44(14) 5_657 2_656
O2 Ba3 O4 102.9(5) 3_665 2_656
O2 Ba3 O4 109.3(4) . 2_656
O2 Ba3 O4 109.3(4) 4_557 2_656
O4 Ba3 O4 120.000(2) 3_666 2_656
O4 Ba3 O4 107.3(17) 1_656 2_656
O4 Ba3 O4 12.7(17) 3_556 2_656
O2 Ba3 O4 102.9(5) 6_667 2_666
O2 Ba3 O4 109.3(4) 2_655 2_666
O2 Ba3 O4 109.3(4) 5_657 2_666
O2 Ba3 O4 102.9(5) 3_665 2_666
O2 Ba3 O4 56.44(14) . 2_666
O2 Ba3 O4 56.44(14) 4_557 2_666
O4 Ba3 O4 107.3(18) 3_666 2_666
O4 Ba3 O4 120.00(4) 1_656 2_666
O4 Ba3 O4 120.00(4) 3_556 2_666
O4 Ba3 O4 132.7(18) 2_656 2_666
O2 Ba3 O4 109.3(4) 6_667 1_556
O2 Ba3 O4 102.9(5) 2_655 1_556
O2 Ba3 O4 102.9(5) 5_657 1_556
O2 Ba3 O4 109.3(4) 3_665 1_556
O2 Ba3 O4 56.44(14) . 1_556
O2 Ba3 O4 56.44(14) 4_557 1_556
O4 Ba3 O4 120.00(4) 3_666 1_556
O4 Ba3 O4 132.7(18) 1_656 1_556
O4 Ba3 O4 107.3(18) 3_556 1_556
O4 Ba3 O4 120.00(4) 2_656 1_556
O4 Ba3 O4 12.7(18) 2_666 1_556
O3 Ba4 O3 120.0 2_765 .
O3 Ba4 O3 120.000(2) 2_765 3_675
O3 Ba4 O3 120.000(5) . 3_675
O3 Ba4 O3 173.3(3) 2_765 2_655
O3 Ba4 O3 53.3(3) . 2_655
O3 Ba4 O3 66.7(3) 3_675 2_655
O3 Ba4 O3 53.3(3) 2_765 3_775
O3 Ba4 O3 66.7(3) . 3_775
O3 Ba4 O3 173.3(3) 3_675 3_775
O3 Ba4 O3 120.0 2_655 3_775
O3 Ba4 O3 66.7(3) 2_765 1_565
O3 Ba4 O3 173.3(3) . 1_565
O3 Ba4 O3 53.3(3) 3_675 1_565
O3 Ba4 O3 120.000(4) 2_655 1_565
O3 Ba4 O3 120.000(5) 3_775 1_565
O3 Ba4 O1 57.44(7) 2_765 2_765
O3 Ba4 O1 92.01(9) . 2_765
O3 Ba4 O1 120.21(12) 3_675 2_765
O3 Ba4 O1 120.21(12) 2_655 2_765
O3 Ba4 O1 57.44(7) 3_775 2_765
O3 Ba4 O1 92.01(9) 1_565 2_765
O3 Ba4 O1 120.21(12) 2_765 4_556
O3 Ba4 O1 57.44(7) . 4_556
O3 Ba4 O1 92.01(9) 3_675 4_556
O3 Ba4 O1 57.44(7) 2_655 4_556
O3 Ba4 O1 92.01(9) 3_775 4_556
O3 Ba4 O1 120.21(12) 1_565 4_556
O1 Ba4 O1 144.95(8) 2_765 4_556
O3 Ba4 O1 120.21(12) 2_765 .
O3 Ba4 O1 57.44(7) . .
O3 Ba4 O1 92.01(9) 3_675 .
O3 Ba4 O1 57.44(7) 2_655 .
O3 Ba4 O1 92.01(9) 3_775 .
O3 Ba4 O1 120.21(12) 1_565 .
O1 Ba4 O1 62.88(16) 2_765 .
O1 Ba4 O1 105.9(2) 4_556 .
O3 Ba4 O1 92.01(9) 2_765 6_676
O3 Ba4 O1 120.21(12) . 6_676
O3 Ba4 O1 57.44(7) 3_675 6_676
O3 Ba4 O1 92.01(9) 2_655 6_676
O3 Ba4 O1 120.21(12) 3_775 6_676
O3 Ba4 O1 57.44(7) 1_565 6_676
O1 Ba4 O1 144.95(8) 2_765 6_676
O1 Ba4 O1 62.88(16) 4_556 6_676
O1 Ba4 O1 144.95(8) . 6_676
O3 Ba4 O1 92.01(9) 2_765 3_675
O3 Ba4 O1 120.21(12) . 3_675
O3 Ba4 O1 57.44(7) 3_675 3_675
O3 Ba4 O1 92.01(9) 2_655 3_675
O3 Ba4 O1 120.21(12) 3_775 3_675
O3 Ba4 O1 57.44(7) 1_565 3_675
O1 Ba4 O1 62.88(16) 2_765 3_675
O1 Ba4 O1 144.95(8) 4_556 3_675
O1 Ba4 O1 62.88(16) . 3_675
O1 Ba4 O1 105.9(2) 6_676 3_675
O3 Ba4 O1 57.44(7) 2_765 5_766
O3 Ba4 O1 92.01(9) . 5_766
O3 Ba4 O1 120.21(12) 3_675 5_766
O3 Ba4 O1 120.21(12) 2_655 5_766
O3 Ba4 O1 57.44(7) 3_775 5_766
O3 Ba4 O1 92.01(9) 1_565 5_766
O1 Ba4 O1 105.9(2) 2_765 5_766
O1 Ba4 O1 62.88(16) 4_556 5_766
O1 Ba4 O1 144.95(8) . 5_766
O1 Ba4 O1 62.88(16) 6_676 5_766
O1 Ba4 O1 144.95(8) 3_675 5_766
O1 Co1 O1 82.2(2) 3_665 2_655
O1 Co1 O1 82.2(2) 3_665 .
O1 Co1 O1 82.2(2) 2_655 .
O1 Co1 O2 94.38(14) 3_665 3_665
O1 Co1 O2 175.4(3) 2_655 3_665
O1 Co1 O2 94.38(14) . 3_665
O1 Co1 O2 94.38(14) 3_665 2_655
O1 Co1 O2 94.38(14) 2_655 2_655
O1 Co1 O2 175.4(2) . 2_655
O2 Co1 O2 88.9(2) 3_665 2_655
O1 Co1 O2 175.4(2) 3_665 .
O1 Co1 O2 94.38(14) 2_655 .
O1 Co1 O2 94.38(14) . .
O2 Co1 O2 88.9(2) 3_665 .
O2 Co1 O2 88.9(2) 2_655 .
O1 Co1 Co2 49.38(15) 3_665 .
O1 Co1 Co2 49.38(15) 2_655 .
O1 Co1 Co2 49.38(15) . .
O2 Co1 Co2 126.05(16) 3_665 .
O2 Co1 Co2 126.05(16) 2_655 .
O2 Co1 Co2 126.05(16) . .
O1 Co1 Ba1 53.84(15) 3_665 1_545
O1 Co1 Ba1 121.22(3) 2_655 1_545
O1 Co1 Ba1 121.22(3) . 1_545
O2 Co1 Ba1 58.12(2) 3_665 1_545
O2 Co1 Ba1 58.12(2) 2_655 1_545
O2 Co1 Ba1 130.73(16) . 1_545
Co2 Co1 Ba1 103.22(2) . 1_545
O1 Co1 Ba1 121.22(3) 3_665 .
O1 Co1 Ba1 121.22(3) 2_655 .
O1 Co1 Ba1 53.84(15) . .
O2 Co1 Ba1 58.12(2) 3_665 .
O2 Co1 Ba1 130.73(16) 2_655 .
O2 Co1 Ba1 58.12(2) . .
Co2 Co1 Ba1 103.22(2) . .
Ba1 Co1 Ba1 114.934(18) 1_545 .
O1 Co1 Ba1 121.22(3) 3_665 1_445
O1 Co1 Ba1 53.84(15) 2_655 1_445
O1 Co1 Ba1 121.22(3) . 1_445
O2 Co1 Ba1 130.73(16) 3_665 1_445
O2 Co1 Ba1 58.12(2) 2_655 1_445
O2 Co1 Ba1 58.12(2) . 1_445
Co2 Co1 Ba1 103.22(2) . 1_445
Ba1 Co1 Ba1 114.934(18) 1_545 1_445
Ba1 Co1 Ba1 114.934(18) . 1_445
O1 Co1 Ba3 130.62(15) 3_665 .
O1 Co1 Ba3 130.62(15) 2_655 .
O1 Co1 Ba3 130.62(15) . .
O2 Co1 Ba3 53.95(16) 3_665 .
O2 Co1 Ba3 53.95(16) 2_655 .
O2 Co1 Ba3 53.95(16) . .
Co2 Co1 Ba3 180.0 . .
Ba1 Co1 Ba3 76.78(2) 1_545 .
Ba1 Co1 Ba3 76.78(2) . .
Ba1 Co1 Ba3 76.78(2) 1_445 .
O1 Co1 Ba2 51.590(16) 3_665 1_545
O1 Co1 Ba2 51.590(16) 2_655 1_545
O1 Co1 Ba2 114.09(16) . 1_545
O2 Co1 Ba2 128.092(17) 3_665 1_545
O2 Co1 Ba2 61.35(15) 2_655 1_545
O2 Co1 Ba2 128.092(17) . 1_545
Co2 Co1 Ba2 64.71(3) . 1_545
Ba1 Co1 Ba2 69.976(9) 1_545 1_545
Ba1 Co1 Ba2 167.93(5) . 1_545
Ba1 Co1 Ba2 69.976(9) 1_445 1_545
Ba3 Co1 Ba2 115.29(3) . 1_545
O1 Co2 O1 83.5(2) 3_665 .
O1 Co2 O1 83.5(2) 3_665 2_655
O1 Co2 O1 83.5(2) . 2_655
O1 Co2 O3 96.15(12) 3_665 3_665
O1 Co2 O3 179.5(2) . 3_665
O1 Co2 O3 96.15(13) 2_655 3_665
O1 Co2 O3 96.15(12) 3_665 .
O1 Co2 O3 96.15(13) . .
O1 Co2 O3 179.5(3) 2_655 .
O3 Co2 O3 84.2(2) 3_665 .
O1 Co2 O3 179.5(2) 3_665 2_655
O1 Co2 O3 96.15(12) . 2_655
O1 Co2 O3 96.15(13) 2_655 2_655
O3 Co2 O3 84.2(2) 3_665 2_655
O3 Co2 O3 84.2(2) . 2_655
O1 Co2 Co2 129.76(14) 3_665 4_556
O1 Co2 Co2 129.76(14) . 4_556
O1 Co2 Co2 129.76(14) 2_655 4_556
O3 Co2 Co2 50.74(16) 3_665 4_556
O3 Co2 Co2 50.74(16) . 4_556
O3 Co2 Co2 50.74(16) 2_655 4_556
O1 Co2 Co1 50.24(14) 3_665 .
O1 Co2 Co1 50.24(14) . .
O1 Co2 Co1 50.24(14) 2_655 .
O3 Co2 Co1 129.26(16) 3_665 .
O3 Co2 Co1 129.26(16) . .
O3 Co2 Co1 129.26(16) 2_655 .
Co2 Co2 Co1 180.0 4_556 .
O1 Co2 Ba2 57.21(2) 3_665 1_655
O1 Co2 Ba2 57.21(2) . 1_655
O1 Co2 Ba2 124.72(15) 2_655 1_655
O3 Co2 Ba2 122.85(3) 3_665 1_655
O3 Co2 Ba2 54.79(15) . 1_655
O3 Co2 Ba2 122.85(3) 2_655 1_655
Co2 Co2 Ba2 105.53(3) 4_556 1_655
Co1 Co2 Ba2 74.47(3) . 1_655
O1 Co2 Ba2 57.21(2) 3_665 1_545
O1 Co2 Ba2 124.72(15) . 1_545
O1 Co2 Ba2 57.21(2) 2_655 1_545
O3 Co2 Ba2 54.79(15) 3_665 1_545
O3 Co2 Ba2 122.85(3) . 1_545
O3 Co2 Ba2 122.85(3) 2_655 1_545
Co2 Co2 Ba2 105.53(3) 4_556 1_545
Co1 Co2 Ba2 74.47(3) . 1_545
Ba2 Co2 Ba2 113.11(2) 1_655 1_545
O1 Co2 Ba2 124.72(15) 3_665 .
O1 Co2 Ba2 57.21(2) . .
O1 Co2 Ba2 57.21(2) 2_655 .
O3 Co2 Ba2 122.85(3) 3_665 .
O3 Co2 Ba2 122.85(3) . .
O3 Co2 Ba2 54.79(15) 2_655 .
Co2 Co2 Ba2 105.53(3) 4_556 .
Co1 Co2 Ba2 74.47(3) . .
Ba2 Co2 Ba2 113.11(2) 1_655 .
Ba2 Co2 Ba2 113.11(2) 1_545 .
O1 Co2 Ba4 59.94(14) 3_665 1_545
O1 Co2 Ba4 125.548(17) . 1_545
O1 Co2 Ba4 125.548(17) 2_655 1_545
O3 Co2 Ba4 54.432(14) 3_665 1_545
O3 Co2 Ba4 54.432(14) . 1_545
O3 Co2 Ba4 120.56(17) 2_655 1_545
Co2 Co2 Ba4 69.82(2) 4_556 1_545
Co1 Co2 Ba4 110.18(2) . 1_545
Ba2 Co2 Ba4 68.909(6) 1_655 1_545
Ba2 Co2 Ba4 68.909(6) 1_545 1_545
Ba2 Co2 Ba4 175.35(5) . 1_545
O4 Co3 O4 22(3) 3_566 2_666
O4 Co3 O4 22(3) 3_566 1_556
O4 Co3 O4 22(3) 2_666 1_556
O4 Co3 O2 102.8(9) 3_566 3_565
O4 Co3 O2 122.4(17) 2_666 3_565
O4 Co3 O2 102.8(9) 1_556 3_565
O4 Co3 O2 102.8(9) 3_566 2_665
O4 Co3 O2 102.8(9) 2_666 2_665
O4 Co3 O2 122.4(17) 1_556 2_665
O2 Co3 O2 109.39(14) 3_565 2_665
O4 Co3 O2 122.4(16) 3_566 .
O4 Co3 O2 102.8(9) 2_666 .
O4 Co3 O2 102.8(9) 1_556 .
O2 Co3 O2 109.39(15) 3_565 .
O2 Co3 O2 109.39(15) 2_665 .
O4 Co3 Ba2 167.1(16) 3_566 .
O4 Co3 Ba2 167.1(17) 2_666 .
O4 Co3 Ba2 167.1(16) 1_556 .
O2 Co3 Ba2 70.45(14) 3_565 .
O2 Co3 Ba2 70.45(14) 2_665 .
O2 Co3 Ba2 70.45(14) . .
O4 Co3 Ba1 93.8(16) 3_566 1_455
O4 Co3 Ba1 112.7(7) 2_666 1_455
O4 Co3 Ba1 112.7(7) 1_556 1_455
O2 Co3 Ba1 56.82(2) 3_565 1_455
O2 Co3 Ba1 56.82(2) 2_665 1_455
O2 Co3 Ba1 143.81(15) . 1_455
Ba2 Co3 Ba1 73.37(2) . 1_455
O4 Co3 Ba1 112.7(7) 3_566 1_445
O4 Co3 Ba1 112.7(7) 2_666 1_445
O4 Co3 Ba1 93.8(16) 1_556 1_445
O2 Co3 Ba1 56.82(2) 3_565 1_445
O2 Co3 Ba1 143.81(15) 2_665 1_445
O2 Co3 Ba1 56.82(2) . 1_445
Ba2 Co3 Ba1 73.37(2) . 1_445
Ba1 Co3 Ba1 112.15(2) 1_455 1_445
O4 Co3 Ba1 112.7(7) 3_566 .
O4 Co3 Ba1 93.8(16) 2_666 .
O4 Co3 Ba1 112.7(7) 1_556 .
O2 Co3 Ba1 143.81(15) 3_565 .
O2 Co3 Ba1 56.82(2) 2_665 .
O2 Co3 Ba1 56.82(2) . .
Ba2 Co3 Ba1 73.37(2) . .
Ba1 Co3 Ba1 112.15(2) 1_455 .
Ba1 Co3 Ba1 112.15(2) 1_445 .
O4 Co3 Ba3 56.3(6) 3_566 1_565
O4 Co3 Ba3 56.3(6) 2_666 1_565
O4 Co3 Ba3 75.0(16) 1_556 1_565
O2 Co3 Ba3 124.96(5) 3_565 1_565
O2 Co3 Ba3 47.47(14) 2_665 1_565
O2 Co3 Ba3 124.96(5) . 1_565
Ba2 Co3 Ba3 117.92(2) . 1_565
Ba1 Co3 Ba3 73.183(9) 1_455 1_565
Ba1 Co3 Ba3 168.72(4) 1_445 1_565
Ba1 Co3 Ba3 73.183(9) . 1_565
O4 Co3 Ba3 56.3(6) 3_566 1_455
O4 Co3 Ba3 75.0(17) 2_666 1_455
O4 Co3 Ba3 56.3(6) 1_556 1_455
O2 Co3 Ba3 47.47(14) 3_565 1_455
O2 Co3 Ba3 124.96(5) 2_665 1_455
O2 Co3 Ba3 124.96(5) . 1_455
Ba2 Co3 Ba3 117.92(2) . 1_455
Ba1 Co3 Ba3 73.183(9) 1_455 1_455
Ba1 Co3 Ba3 73.183(9) 1_445 1_455
Ba1 Co3 Ba3 168.72(4) . 1_455
Ba3 Co3 Ba3 99.86(3) 1_565 1_455
Co2 O1 Co1 80.4(2) . .
Co2 O1 Ba1 171.8(2) . .
Co1 O1 Ba1 91.45(16) . .
Co2 O1 Ba2 88.98(10) . 1_655
Co1 O1 Ba2 96.72(10) . 1_655
Ba1 O1 Ba2 92.00(10) . 1_655
Co2 O1 Ba2 88.98(10) . .
Co1 O1 Ba2 96.72(10) . .
Ba1 O1 Ba2 92.00(10) . .
Ba2 O1 Ba2 165.87(17) 1_655 .
Co2 O1 Ba4 87.27(15) . .
Co1 O1 Ba4 167.7(2) . .
Ba1 O1 Ba4 100.89(17) . .
Ba2 O1 Ba4 82.97(9) 1_655 .
Ba2 O1 Ba4 82.97(9) . .
Co3 O2 Co1 163.5(3) . .
Co3 O2 Ba3 104.25(17) . .
Co1 O2 Ba3 92.3(2) . .
Co3 O2 Ba1 91.17(14) . 1_445
Co1 O2 Ba1 86.75(11) . 1_445
Ba3 O2 Ba1 96.99(10) . 1_445
Co3 O2 Ba1 91.17(14) . .
Co1 O2 Ba1 86.75(11) . .
Ba3 O2 Ba1 96.99(10) . .
Ba1 O2 Ba1 164.80(17) 1_445 .
Co3 O2 Ba2 77.14(19) . .
Co1 O2 Ba2 86.36(14) . .
Ba3 O2 Ba2 178.6(2) . .
Ba1 O2 Ba2 82.94(10) 1_445 .
Ba1 O2 Ba2 82.94(10) . .
Co2 O3 Co2 78.5(3) 4_556 .
Co2 O3 Ba2 169.7(3) 4_556 1_655
Co2 O3 Ba2 91.20(5) . 1_655
Co2 O3 Ba2 91.20(5) 4_556 4_656
Co2 O3 Ba2 169.7(3) . 4_656
Ba2 O3 Ba2 99.1(2) 1_655 4_656
Co2 O3 Ba4 92.58(12) 4_556 .
Co2 O3 Ba4 92.58(12) . .
Ba2 O3 Ba4 87.84(11) 1_655 .
Ba2 O3 Ba4 87.84(11) 4_656 .
Co2 O3 Ba4 92.58(12) 4_556 1_545
Co2 O3 Ba4 92.58(12) . 1_545
Ba2 O3 Ba4 87.84(11) 1_655 1_545
Ba2 O3 Ba4 87.84(11) 4_656 1_545
Ba4 O3 Ba4 173.3(3) . 1_545
O4 O4 O4 60.000(6) 2_665 3_565
O4 O4 Co3 78.9(14) 2_665 4_556
O4 O4 Co3 78.9(14) 3_565 4_556
O4 O4 Co3 78.9(14) 2_665 1_554
O4 O4 Co3 78.9(14) 3_565 1_554
Co3 O4 Co3 154(3) 4_556 1_554
O4 O4 Ba3 143.6(9) 2_665 1_454
O4 O4 Ba3 83.6(9) 3_565 1_454
Co3 O4 Ba3 95.1(5) 4_556 1_454
Co3 O4 Ba3 95.1(5) 1_554 1_454
O4 O4 Ba3 83.6(9) 2_665 1_554
O4 O4 Ba3 143.6(9) 3_565 1_554
Co3 O4 Ba3 95.1(5) 4_556 1_554
Co3 O4 Ba3 95.1(5) 1_554 1_554
Ba3 O4 Ba3 132.7(17) 1_454 1_554
Ba1 F1 Ba1 180.0 4_557 .
Ba1 F1 Ba3 90.0 4_557 1_565
Ba1 F1 Ba3 90.0 . 1_565
Ba1 F1 Ba3 90.0 4_557 1_665
Ba1 F1 Ba3 90.0 . 1_665
Ba3 F1 Ba3 120.0 1_565 1_665
Ba1 F1 Ba3 90.0 4_557 .
Ba1 F1 Ba3 90.0 . .
Ba3 F1 Ba3 120.0 1_565 .
Ba3 F1 Ba3 120.0 1_665 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ba1 F1 2.7116(9) .
Ba1 O1 2.715(5) .
Ba1 O1 2.715(5) 3_675
Ba1 O1 2.715(5) 2_765
Ba1 O2 2.8593(6) 1_665
Ba1 O2 2.8593(6) .
Ba1 O2 2.8593(6) 2_765
Ba1 O2 2.8593(6) 3_675
Ba1 O2 2.8593(6) 3_665
Ba1 O2 2.8593(6) 2_665
Ba1 Co1 3.3616(4) 1_565
Ba1 Co1 3.3616(4) .
Ba2 O3 2.776(5) 1_455
Ba2 O3 2.776(5) 3_675
Ba2 O3 2.776(5) 2_655
Ba2 O1 2.8558(6) 3_675
Ba2 O1 2.8558(6) 2_665
Ba2 O1 2.8558(6) 1_455
Ba2 O1 2.8558(6) 3_565
Ba2 O1 2.8558(6) 2_655
Ba2 O1 2.8558(6) .
Ba2 O2 3.183(5) 2_665
Ba2 O2 3.183(5) 3_565
Ba2 O2 3.183(5) .
Ba3 O2 2.816(5) 6_667
Ba3 O2 2.816(5) 2_655
Ba3 O2 2.816(5) 5_657
Ba3 O2 2.816(5) 3_665
Ba3 O2 2.816(5) .
Ba3 O2 2.816(5) 4_557
Ba3 O4 3.09(2) 3_666
Ba3 O4 3.09(2) 1_656
Ba3 O4 3.09(2) 3_556
Ba3 O4 3.09(2) 2_656
Ba3 O4 3.09(2) 2_666
Ba3 O4 3.09(2) 1_556
Ba4 O3 2.8390(5) 2_765
Ba4 O3 2.8390(5) .
Ba4 O3 2.8390(5) 3_675
Ba4 O3 2.8390(5) 2_655
Ba4 O3 2.8390(5) 3_775
Ba4 O3 2.8390(5) 1_565
Ba4 O1 3.021(4) 2_765
Ba4 O1 3.021(4) 4_556
Ba4 O1 3.021(4) .
Ba4 O1 3.021(4) 6_676
Ba4 O1 3.021(4) 3_675
Ba4 O1 3.021(4) 5_766
Co1 O1 1.915(5) 3_665
Co1 O1 1.915(5) 2_655
Co1 O1 1.915(5) .
Co1 O2 1.938(6) 3_665
Co1 O2 1.938(6) 2_655
Co1 O2 1.938(6) .
Co1 Co2 2.456(2) .
Co1 Ba1 3.3616(4) 1_545
Co1 Ba1 3.3616(4) 1_445
Co1 Ba2 3.6195(8) 1_545
Co2 O1 1.890(5) 3_665
Co2 O1 1.890(5) .
Co2 O1 1.890(5) 2_655
Co2 O3 1.900(6) 3_665
Co2 O3 1.900(6) .
Co2 O3 1.900(6) 2_655
Co2 Co2 2.405(3) 4_556
Co2 Ba2 3.3965(5) 1_655
Co2 Ba2 3.3965(5) 1_545
Co2 Ba4 3.4866(6) 1_545
Co3 O4 1.779(11) 3_566
Co3 O4 1.779(12) 2_666
Co3 O4 1.779(12) 1_556
Co3 O2 1.811(7) 3_565
Co3 O2 1.811(7) 2_665
Co3 O2 1.811(6) .
Co3 Ba1 3.4155(5) 1_455
Co3 Ba1 3.4155(5) 1_445
Co3 Ba3 3.7035(7) 1_565
Co3 Ba3 3.7035(7) 1_455
O1 Ba2 2.8558(6) 1_655
O2 Ba1 2.8593(6) 1_445
O3 Co2 1.900(6) 4_556
O3 Ba2 2.776(5) 1_655
O3 Ba2 2.776(5) 4_656
O3 Ba4 2.8390(5) 1_545
O4 O4 0.69(9) 2_665
O4 O4 0.69(9) 3_565
O4 Co3 1.779(11) 4_556
O4 Co3 1.779(11) 1_554
O4 Ba3 3.09(2) 1_454
O4 Ba3 3.09(2) 1_554
F1 Ba1 2.7116(9) 4_557
F1 Ba3 3.2726(3) 1_565
F1 Ba3 3.2726(3) 1_665
